Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- Mechanics of Materials 5th edition ... by Noor Aldin Zghoul 147015 views
- Strength of materials by s k mondal by Shubhra Saxena 146991 views
- Timoshenko strength-of-materials by Dr. Haider alsenisal 951 views
- Mechanics.of.materials.gere.6th.ch0... by Lpvince 5927 views
- Elements of Solid Mechanics.ppt by Daffodil Internat... 500 views
- Mechanics of materials solution man... by Pawnpac 194690 views

1,628 views

1,443 views

1,443 views

Published on

No Downloads

Total views

1,628

On SlideShare

0

From Embeds

0

Number of Embeds

1

Shares

0

Downloads

0

Comments

0

Likes

3

No embeds

No notes for slide

- 1. INTRODUCTION AND REVIEW Preamble Engineering science is usually subdivided into number of topics such as 1. Solid Mechanics 2. Fluid Mechanics 3. Heat Transfer 4. Properties of materials and soon Although there are close links between them in terms of the physical principles involved and methods of analysis employed. The solid mechanics as a subject may be defined as a branch of applied mechanics that deals with behaviors of solid bodies subjected to various types of loadings. This is usually subdivided into further two streams i.e. Mechanics of rigid bodies or simply Mechanics and Mechanics of deformable solids. The mechanics of deformable solids which is branch of applied mechanics is known by several names i.e. strength of materials, mechanics of materials etc. Mechanics of rigid bodies: The mechanics of rigid bodies is primarily concerned with the static and dynamic behaviour under external forces of engineering components and systems which are treated as infinitely strong and undeformable primarily we deal here with the forces and motions associated with particles and rigid bodies. Mechanics of deformable solids: Mechanics of solids: The mechanics of deformable solids is more concerned with the internal forces and associated changes in the geometry of the components involved. Of particular importance are the properties of the materials used, the strength of which will determine whether the components fail by breaking in service, and the stiffness of which will determine whether the amount of deformation they suffer is acceptable. Therefore, the subject of mechanics of materials or strength of materials is central to the whole activity of engineering design. Usually the objectives in analysis here will be the determination of the stresses, strains, and deflections produced by loads. Theoretical analyses and experimental results have an equal roles in this field. Analysis of stress and strain: Concept of stress: Let us introduce the concept of stress as we know that the main problem of engineering mechanics of material is the investigation of the internal resistance of the body, i.e. the nature of forces set up within a body to balance the effect of the externally applied forces.
- 2. The externally applied forces are termed as loads. These externally applied forces may be due to any one of the reason. (i) due to service conditions (ii) due to environment in which the component works (iii) through contact with other members (iv) due to fluid pressures (v) due to gravity or inertia forces. As we know that in mechanics of deformable solids, externally applied forces acts on a body and body suffers a deformation. From equilibrium point of view, this action should be opposed or reacted by internal forces which are set up within the particles of material due to cohesion. These internal forces give rise to a concept of stress. Therefore, let us define a stress Therefore; let us define a term stress Stress: Let us consider a rectangular bar of some cross – sectional area and subjected to some load or force (in Newtons) Let us imagine that the same rectangular bar is assumed to be cut into two halves at section XX. The each portion of this rectangular bar is in equilibrium under the action of load P and the internal forces acting at the section XX has been shown
- 3. Now stress is defined as the force intensity or force per unit area. Here we use a symbol to represent the stress. Where A is the area of the X – section Here we are using an assumption that the total force or total load carried by the rectangular bar is uniformly distributed over its cross – section. But the stress distributions may be for from uniform, with local regions of high stress known as stress concentrations. If the force carried by a component is not uniformly distributed over its cross – sectional area, A, we must consider a small area, ‘A' which carries a small load P, of the total force ‘P', Then definition of stress is As a particular stress generally holds true only at a point, therefore it is defined mathematically as Units : The basic units of stress in S.I units i.e. (International system) are N / m2 (or Pa) MPa = 106 Pa GPa = 109 Pa KPa = 103 Pa Some times N / mm2 units are also used, because this is an equivalent to MPa. While US customary unit is pound per square inch psi.
- 4. TYPES OF STRESSES : Only two basic stresses exists : (1) normal stress and (2) shear stress. Other stresses either are similar to these basic stresses or are a combination of this e.g. bending stress is a combination tensile, compressive and shear stresses. Torsional stress, as encountered in twisting of a shaft is a shearing stress. Let us define the normal stresses and shear stresses in the following sections. Normal stresses: We have defined stress as force per unit area. If the stresses are normal to the areas concerned, then these are termed as normal stresses. The normal stresses are generally denoted by a Greek letter ( ) This is also known as uniaxial state of stress, because the stresses acts only in one direction however, such a state rarely exists, therefore we have biaxial and triaxial state of stresses where either the two mutually perpendicular normal stresses acts or three mutually perpendicular normal stresses acts as shown in the figures below :
- 5. Tensile or compressive stresses : The normal stresses can be either tensile or compressive whether the stresses acts out of the area or into the area Bearing Stress: When one object presses against another, it is referred to a bearing stress ( They are in fact the compressive stresses ).
- 6. Shear stresses: Let us consider now the situation, where the cross – sectional area of a block of material is subject to a distribution of forces which are parallel, rather than normal, to the area concerned. Such forces are associated with a shearing of the material, and are referred to as shear forces. The resulting force interistes are known as shear stresses. The resulting force intensities are known as shear stresses, the mean shear stress being equal to Where P is the total force and A the area over which it acts. As we know that the particular stress generally holds good only at a point therefore we can define shear stress at a point as The greek symbol ( tau ) ( suggesting tangential ) is used to denote shear stress. However, it must be borne in mind that the stress ( resultant stress ) at any point in a body is basically resolved into two components and one acts perpendicular and other parallel to the area concerned, as it is clearly defined in the following figure.
- 7. The single shear takes place on the single plane and the shear area is the cross - sectional of the rivet, whereas the double shear takes place in the case of Butt joints of rivets and the shear area is the twice of the X - sectional area of the rivet.
- 8. ANALYSIS OF STERSSES General State of stress at a point: Stress at a point in a material body has been defined as a force per unit area. But this definition is some what ambiguous since it depends upon what area we consider at that point. Let us, consider a point ‘q' in the interior of the body Let us pass a cutting plane through a pont 'q' perpendicular to the x - axis as shown below The corresponding force components can be shown like this dFx = xx. dax dFy = xy. dax dFz = xz. dax where dax is the area surrounding the point 'q' when the cutting plane r is to x - axis. In a similar way it can be assummed that the cutting plane is passed through the point 'q' perpendicular to the y - axis. The corresponding force components are shown below
- 9. The corresponding force components may be written as dFx = yx. day dFy = yy. day dFz = yz. day where day is the area surrounding the point 'q' when the cutting plane r is to y - axis. In the last it can be considered that the cutting plane is passed through the point 'q' perpendicular to the z - axis. The corresponding force components may be written as dFx = zx. daz dFy = zy. daz dFz = zz. daz Where daz is the area surrounding the point 'q' when the cutting plane r is to z - axis. Thus, from the foregoing discussion it is amply clear that there is nothing like stress at a point 'q' rather we have a situation where it is a combination of state of stress at a point q. Thus, it becomes imperative to understand the term state of stress at a point 'q'. Therefore, it becomes easy to express astute of stress by the scheme as discussed earlier, where the stresses on the three mutually perpendicular planes are labeled in the manner as shown earlier. the state of stress as depicted earlier is called the general or a triaxial state of stress that can exist at any interior point of a loaded body. Before defining the general state of stress at a point. Let us make overselves conversant with the notations for the stresses. We have already chosen to distinguish between normal and shear stress with the help of symbols and .
- 10. Cartesian - co-ordinate system In the Cartesian co-ordinates system, we make use of the axes, X, Y and Z Let us consider the small element of the material and show the various normal stresses acting the faces Thus, in the Cartesian co-ordinates system the normal stresses have been represented by x, yand z. Cylindrical - co-ordinate system In the Cylindrical - co-ordinate system we make use of co-ordinates r, and Z. Thus, in the Cylindrical co-ordinates system, the normal stresses i.e components acting over a element is being denoted by r, and z. Sign convention : The tensile forces are termed as ( +ve ) while the compressive forces are termed as negative ( -ve ). First sub – script : it indicates the direction of the normal to the surface. Second subscript : it indicates the direction of the stress.
- 11. It may be noted that in the case of normal stresses the double script notation may be dispensed with as the direction of the normal stress and the direction of normal to the surface of the element on which it acts is the same. Therefore, a single subscript notation as used is sufficient to define the normal stresses. Shear Stresses : With shear stress components, the single subscript notation is not practical, because such stresses are in direction parallel to the surfaces on which they act. We therefore have two directions to specify, that of normal to the surface and the stress itself. To do this, we stress itself. To do this, we attach two subscripts to the symbol ' ' , for shear stresses. In Cartesian and polar co-ordinates, we have the stress components as shown in the figures. xy , yx , yz , zy , zx , xz r , r , z , z ,zr , rz So as shown above, the normal stresses and shear stress components indicated on a small element of material separately has been combined and depicted on a single element. Similarly for a cylindrical co-ordinate system let us shown the normal and shear stresses components separately.
- 12. Now let us combine the normal and shear stress components as shown below : Now let us define the state of stress at a point formally. State of stress at a point :
- 13. By state of stress at a point, we mean an information which is required at that point such that it remains under equilibrium. or simply a general state of stress at a point involves all the normal stress components, together with all the shear stress components as shown in earlier figures. Therefore, we need nine components, to define the state of stress at a point x xy xz y yx yz z zx zy If we apply the conditions of equilibrium which are as follows: Fx = 0 ; M x = 0 Fy = 0 ; M y = 0 Fz = 0 ; M z = 0 Then we get xy = yx yz = zy zx = xy Then we will need only six components to specify the state of stress at a point i.e x , y, z , xy , yz , zx Now let us define the concept of complementary shear stresses. Complementary shear stresses: The existence of shear stresses on any two sides of the element induces complementary shear stresses on the other two sides of the element to maintain equilibrium.
- 14. On planes AB and CD, the shear stress acts. To maintain the static equilibrium of this element, on planes AD and BC, ' should act, we shall see that ' which is known as the complementary shear stress would come out to equal and opposite to the. Let us prove this thing for a general case as discussed below: The figure shows a small rectangular element with sides of length x, y parallel to x and y directions. Its thickness normal to the plane of paper isz in z – direction. All nine normal and shear stress components may act on the element, only those in x and y directions are shown. Sign convections for shear stresses: Direct stresses or normal stresses - tensile +ve - compressive –ve Shear stresses: - tending to turn the element C.W +ve. - tending to turn the element C.C.W – ve. The resulting forces applied to the element are in equilibrium in x and y direction. ( Although other normal and shear stress components are not shown, their presence does not affect the final conclusion ). Assumption : The weight of the element is neglected. Since the element is a static piece of solid body, the moments applied to it must also be in equilibrium. Let ‘O' be the centre of the element. Let us consider the axis through the point ‘O'. the resultant force associated with normal stresses x and y acting on the sides of the element each pass through this axis, and therefore, have no moment.
- 15. Now forces on top and bottom surfaces produce a couple which must be balanced by the forces on left and right hand faces Thus, yx . x . z . y = xy . x . z . y In other word, the complementary shear stresses are equal in magnitude. The same form of relationship can be obtained for the other two pair of shear stress components to arrive at the relations
- 16. Analysis of Stresses: Consider a point ‘q' in some sort of structural member like as shown in figure below. Assuming that at point exist. ‘q' a plane state of stress exist. i.e. the state of state stress is to describe by a parameters x, y and xy These stresses could be indicate a on the two dimensional diagram as shown below: This is a commen way of representing the stresses. It must be realize a that the material is unaware of what we have called the x and y axes. i.e. the material has to resist the loads irrespective less of how we wish to name them or whether they are horizontal, vertical or otherwise further more, the material will fail when the stresses exceed beyond a permissible value. Thus, a fundamental problem in engineering design is to determine the maximum normal stress or maximum shear stress at any particular point in a body. There is no reason to believe apriori that x, y and xy are the maximum value. Rather the maximum stresses may associates themselves with some other planes located at ‘'. Thus, it becomes imperative to determine the values of and. In order tto achieve this let us consider the following.
- 17. Shear stress: If the applied load P consists of two equal and opposite parallel forces not in the same line, than there is a tendency for one part of the body to slide over or shear from the other part across any section LM. If the cross section at LM measured parallel to the load is A, then the average value of shear stress = P/A . The shear stress is tangential to the area over which it acts. If the shear stress varies then at a point then may be defined as Complementary shear stress: Let ABCD be a small rectangular element of sides x, y and z perpendicular to the plane of paper let there be shear stress acting on planes AB and CD It is obvious that these stresses will from a couple ( . xz )y which can only be balanced by tangential forces on planes AD and BC. These are known as complementary shear stresses. i.e. the existence of shear stresses on sides AB and CD of the element implies that there must also be complementary shear stresses on to maintain equilibrium. Let ' be the complementary shear stress induced on planes AD and BC. Then for the equilibrium (. xz )y = ' ( yz )x = ' Thus, every shear stress is accompanied by an equal complementary shear stress. Stresses on oblique plane: Till now we have dealt with either pure normal direct stress or pure shear stress. In many instances, however both direct and shear stresses acts and the resultant stress across any section will be neither normal nor tangential to the plane.
- 18. A plane stse of stress is a 2 dimensional stae of stress in a sense that the stress components in one direction are all zero i.e z = yz = zx = 0 examples of plane state of stress includes plates and shells. Consider the general case of a bar under direct load F giving rise to a stress y vertically The stress acting at a point is represented by the stresses acting on the faces of the element enclosing the point. The stresses change with the inclination of the planes passing through that point i.e. the stress on the faces of the element vary as the angular position of the element changes. Let the block be of unit depth now considering the equilibrium of forces on the triangle portion ABC Resolving forces perpendicular to BC, gives .BC.1 = ysin . AB . 1 but AB/BC = sin or AB = BCsin Substituting this value in the above equation, we get .BC.1 = ysin . BCsin . 1 or (1) Now resolving the forces parallel to BC .BC.1 = y cos . ABsin . 1
- 19. again AB = BCcos .BC.1 = ycos . BCsin . 1 or = ysincos (2) If = 900 the BC will be parallel to AB and = 0, i.e. there will be only direct stress or normal stress. By examining the equations (1) and (2), the following conclusions may be drawn (i) The value of direct stress is maximum and is equal to y when = 900 . (ii) The shear stress has a maximum value of 0.5 y when = 450 (iii) The stresses and are not simply the resolution of y Material subjected to pure shear: Consider the element shown to which shear stresses have been applied to the sides AB and DC Complementary shear stresses of equal value but of opposite effect are then set up on the sides AD and BC in order to prevent the rotation of the element. Since the applied and complementary shear stresses are of equal value on the x and y planes. Therefore, they are both represented by the symbol xy. Now consider the equilibrium of portion of PBC
- 20. Assuming unit depth and resolving normal to PC or in the direction of .PC.1 =xy.PB.cos.1+xy.BC.sin.1 = xy.PB.cos + xy.BC.sin Now writing PB and BC in terms of PC so that it cancels out from the two sides PB/PC = sin BC/PC = cos .PC.1 = xy.cossinPC+ xy.cos.sinPC = 2xysincos = xy.2.sincos (1) Now resolving forces parallel to PC or in the direction .then xyPC . 1 =xy . PBsin xy . BCcos ve sign has been put because this component is in the same direction as that of . again converting the various quantities in terms of PC we have xyPC . 1 =xy . PB.sin2 xy . PCcos2 = [xy (cos2 sin2 ) ] = xycos2or (2) the negative sign means that the sense of is opposite to that of assumed one. Let us examine the equations (1) and (2) respectively
- 21. From equation (1) i.e, = xy sin2 The equation (1) represents that the maximum value of isxy when = 450 . Let us take into consideration the equation (2) which states that =xy cos2 It indicates that the maximum value of isxy when = 00 or 900 . it has a value zero when = 450 . From equation (1) it may be noticed that the normal component has maximum and minimum values of +xy (tension) and xy (compression) on plane at ± 450 to the applied shear and on these planes the tangential component is zero. Hence the system of pure shear stresses produces and equivalent direct stress system, one set compressive and one tensile each located at 450 to the original shear directions as depicted in the figure below: Material subjected to two mutually perpendicular direct stresses: Now consider a rectangular element of unit depth, subjected to a system of two direct stresses both tensile, x and yacting right angles to each other.
- 22. for equilibrium of the portion ABC, resolving perpendicular to AC . AC.1 = y sin . AB.1 + x cos . BC.1 converting AB and BC in terms of AC so that AC cancels out from the sides = y sin2 + xcos2 Futher, recalling that cos2 sin2 = cos2 or (1 cos2)/2 = sin2 Similarly (1 + cos2)/2 = cos2 q Hence by these transformations the expression for reduces to = 1/2y (1 cos2) + 1/2x (1 + cos2) On rearranging the various terms we get (3) Now resolving parallal to AC sq.AC.1= xy..cos.AB.1+xy.BC.sin.1 The – ve sign appears because this component is in the same direction as that of AC. Again converting the various quantities in terms of AC so that the AC cancels out from the two sides.
- 23. (4) Conclusions : The following conclusions may be drawn from equation (3) and (4) (i) The maximum direct stress would be equal to x or y which ever is the greater, when = 00 or 900 (ii) The maximum shear stress in the plane of the applied stresses occurs when = 450 Material subjected to combined direct and shear stresses: Now consider a complex stress system shown below, acting on an element of material. The stresses x and y may be compressive or tensile and may be the result of direct forces or as a result of bending.The shear stresses may be as shown or completely reversed and occur as a result of either shear force or torsion as shown in the figure below: As per the double subscript notation the shear stress on the face BC should be notified as yx , however, we have already seen that for a pair of shear stresses there is a set of complementary shear stresses generated such that yx = xy
- 24. By looking at this state of stress, it may be observed that this state of stress is combination of two different cases: (i) Material subjected to pure stae of stress shear. In this case the various formulas deserved are as follows = yx sin2 = yx cos 2 (ii) Material subjected to two mutually perpendicular direct stresses. In this case the various formula's derived are as follows. To get the required equations for the case under consideration,let us add the respective equations for the above two cases such that These are the equilibrium equations for stresses at a point. They do not depend on material proportions and are equally valid for elastic and inelastic behaviour This eqn gives two values of 2 that differ by 1800 .Hence the planes on which maximum and minimum normal stresses occurate 900 apart.
- 25. From the triangle it may be determined Substituting the values of cos2and sin2in equation (5) we get
- 26. This shows that the values oshear stress is zero on the principal planes. Hence the maximum and minimum values of normal stresses occur on planes of zero shearing stress. The maximum and minimum normal stresses are called the principal stresses, and the planes on which they act are called principal plane the solution of equation
- 27. will yield two values of 2 separated by 1800 i.e. two values of separated by 900 .Thus the two principal stresses occur on mutually perpendicular planes termed principal planes. Therefore the two – dimensional complex stress system can now be reduced to the equivalent system of principal stresses. Let us recall that for the case of a material subjected to direct stresses the value of maximum shear stresses
- 28. Therefore,it can be concluded that the equation (2) is a negative reciprocal of equation (1) hence the roots for the double angle of equation (2) are 900 away from the corresponding angle of equation (1). This means that the angles that angles that locate the plane of maximum or minimum shearing stresses form angles of 450 with the planes of principal stresses. Futher, by making the triangle we get Because of root the difference in sign convention arises from the point of view of locating the planes on which shear stress act. From physical point of view these sign have no meaning. The largest stress regard less of sign is always know as maximum shear stress. Principal plane inclination in terms of associated principal stress: We know that the equation yields two values of q i.e. the inclination of the two principal planes on which the principal stresses s1 and s2 act. It is uncertain,however, which stress acts on which plane unless equation.
- 29. is used and observing which one of the two principal stresses is obtained. Alternatively we can also find the answer to this problem in the following manner Consider once again the equilibrium of a triangular block of material of unit depth, Assuming AC to be a principal plane on which principal stressesp acts, and the shear stress is zero. Resolving the forces horizontally we get: x .BC . 1 + xy .AB . 1 = p . cos . AC dividing the above equation through by BC we get
- 30. GRAPHICAL SOLUTION – MOHR'S STRESS CIRCLE The transformation equations for plane stress can be represented in a graphical form known as Mohr's circle. This grapical representation is very useful in depending the relationships between normal and shear stresses acting on any inclined plane at a point in a stresses body. To draw a Mohr's stress circle consider a complex stress system as shown in the figure The above system represents a complete stress system for any condition of applied load in two dimensions The Mohr's stress circle is used to find out graphically the direct stress and sheer stresson any plane inclined at to the plane on which xacts.The direction of here is taken in anticlockwise direction from the BC. STEPS: In order to do achieve the desired objective we proceed in the following manner (i) Label the Block ABCD. (ii) Set up axes for the direct stress (as abscissa) and shear stress (as ordinate) (iii) Plot the stresses on two adjacent faces e.g. AB and BC, using the following sign convention. Direct stressestensile positive; compressive, negative Shear stresses – tending to turn block clockwise, positive – tending to turn block counter clockwise, negative [ i.e shearing stresses are +ve when its movement about the centre of the element is clockwise ]
- 31. This gives two points on the graph which may than be labeled as respectively to denote stresses on these planes. (iv) Join . (v) The point P where this line cuts the s axis is than the centre of Mohr's stress circle and the line joining is diameter. Therefore the circle can now be drawn. Now every point on the circle then represents a state of stress on some plane through C. Proof:
- 32. Consider any point Q on the circumference of the circle, such that PQ makes an angle 2with BC, and drop a perpendicular from Q to meet the s axis at N.Then OQ represents the resultant stress on the plane an angle to BC. Here we have assumed that x y Now let us find out the coordinates of point Q. These are ON and QN. From the figure drawn earlier ON = OP + PN OP = OK + KP OP = y + 1/2 ( xy) = y / 2 + y / 2 + x / 2 + y / 2 = ( x + y ) / 2 PN = Rcos( 2 ) hence ON = OP + PN = ( x + y ) / 2 + Rcos( 2) = (x + y ) / 2 + Rcos2 cos + Rsin2sin now make the substitutions for Rcos and Rsin.
- 33. Thus, ON = 1/2 (x + y ) + 1/2 (x y )cos2 + xysin2 (1) Similarly QM = Rsin( 2 ) = Rsin2cos - Rcos2sin Thus, substituting the values of R cos and Rsin, we get QM = 1/2 ( x y)sin2 xycos2 (2) If we examine the equation (1) and (2), we see that this is the same equation which we have already derived analytically Thus the co-ordinates of Q are the normal and shear stresses on the plane inclined at to BC in the original stress system. N.B: Since angle PQ is 2 on Mohr's circle and not it becomes obvious that angles are doubled on Mohr's circle. This is the only difference, however, as They are measured in the same direction and from the same plane in both figures. Further points to be noted are : (1) The direct stress is maximum when Q is at M and at this point obviously the sheer stress is zero, hence by definition OM is the length representing the maximum principal stresses 1 and 21 gives the angle of the plane 1 from BC. Similar OL is the other principal stress and is represented by 2 (2) The maximum shear stress is given by the highest point on the circle and is represented by the radius of the circle. This follows that since shear stresses and complimentary sheer stresses have the same value; therefore the centre of the circle will always lie on the s axis midway between x and y . [ since +xy & xy are shear stress & complimentary shear stress so they are same in magnitude but different in sign. ] (3) From the above point the maximum sheer stress i.e. the Radius of the Mohr's stress circle would be While the direct stress on the plane of maximum shear must be mid – may between x and y i.e
- 34. (4) As already defined the principal planes are the planes on which the shear components are zero. Therefore are conclude that on principal plane the sheer stress is zero. (5) Since the resultant of two stress at 900 can be found from the parallogram of vectors as shown in the diagram.Thus, the resultant stress on the plane at q to BC is given by OQ on Mohr's Circle. (6) The graphical method of solution for a complex stress problems using Mohr's circle is a very powerful technique, since all the information relating to any plane within the stressed element is contained in the single construction. It thus, provides a convenient and rapid means of solution. Which is less prone to arithmetical errors and is highly recommended. ILLUSRATIVE PROBLEMS: Let us discuss few representative problems dealing with complex state of stress to be solved either analytically or graphically. PROB 1: A circular bar 40 mm diameter carries an axial tensile load of 105 kN. What is the Value of shear stress on the planes on which the normal stress has a value of 50 MN/m2 tensile. Solution:
- 35. Tensile stress y= F / A = 105 x 103 / x (0.02)2 = 83.55 MN/m2 Now the normal stress on an obliqe plane is given by the relation = ysin2 50 x 106 = 83.55 MN/m2 x 106 sin2 = 500 68' The shear stress on the oblique plane is then given by = 1/2 ysin2 = 1/2 x 83.55 x 106 x sin 101.36 = 40.96 MN/m2 Therefore the required shear stress is 40.96 MN/m2 PROB 2: For a given loading conditions the state of stress in the wall of a cylinder is expressed as follows: (a) 85 MN/m2 tensile (b) 25 MN/m2 tensile at right angles to (a) (c) Shear stresses of 60 MN/m2 on the planes on which the stresses (a) and (b) act; the sheer couple acting on planes carrying the 25 MN/m2 stress is clockwise in effect. Calculate the principal stresses and the planes on which they act. What would be the effect on these results if owing to a change of loading (a) becomes compressive while stresses (b) and (c) remain unchanged Solution: The problem may be attempted both analytically as well as graphically. Let us first obtain the analytical solution
- 36. The principle stresses are given by the formula For finding out the planes on which the principle stresses act us the equation The solution of this equation will yeild two values i.e they 1 and 2 giving 1= 310 71' & 2= 1210 71' (b) In this case only the loading (a) is changed i.e. its direction had been changed. While the other stresses remains unchanged hence now the block diagram becomes.
- 37. Again the principal stresses would be given by the equation. Thus, the two principle stresses acting on the two mutually perpendicular planes i.e principle planes may be depicted on the element as shown below: So this is the direction of one principle plane & the principle stresses acting on this would be 1 when is acting normal to this plane, now the direction of other principal plane would be 900 + because the principal planes are the two mutually perpendicular plane, hence rotate the another plane + 900 in the same direction to get the another plane, now complete the material element if is negative that means we are measuring the angles in the opposite direction to the reference plane BC .
- 38. Therefore the direction of other principal planes would be { + 90} since the angle is always less in magnitude then 90 hence the quantity (+ 90 ) would be positive therefore the Inclination of other plane with reference plane would be positive therefore if just complete the Block. It would appear as If we just want to measure the angles from the reference plane, than rotate this block through 1800 so as to have the following appearance. So whenever one of the angles comes negative to get the positive value,
- 39. first Add 900 to the value and again add 900 as in this case = 230 74' so 1 = 230 74' + 900 = 660 26' .Again adding 900 also gives the direction of other principle planes i.e 2 = 660 26' + 900 = 1560 26' This is how we can show the angular position of these planes clearly. GRAPHICAL SOLUTION: Mohr's Circle solution: The same solution can be obtained using the graphical solution i.e the Mohr's stress circle,for the first part, the block diagram becomes Construct the graphical construction as per the steps given earlier. Taking the measurements from the Mohr's stress circle, the various quantities computed are
- 40. 1 = 120 MN/m2 tensile 2 = 10 MN/m2 compressive 1 = 340 counter clockwise from BC 2 = 340 + 90 = 1240 counter clockwise from BC Part Second : The required configuration i.e the block diagram for this case is shown along with the stress circle. By taking the measurements, the various quantites computed are given as 1 = 56.5 MN/m2 tensile 2 = 106 MN/m2 compressive 1 = 660 15' counter clockwise from BC 2 = 1560 15' counter clockwise from BC Salient points of Mohr's stress circle: 1. complementary shear stresses (on planes 900 apart on the circle) are equal in magnitude 2. The principal planes are orthogonal: points L and M are 1800 apart on the circle (900 apart in material) 3. There are no shear stresses on principal planes: point L and M lie on normal stress axis.
- 41. 4. The planes of maximum shear are 450 from the principal points D and E are 900 , measured round the circle from points L and M. 5. The maximum shear stresses are equal in magnitude and given by points D and E 6. The normal stresses on the planes of maximum shear stress are equal i.e. points D and E both have normal stress co-ordinate which is equal to the two principal stresses. As we know that the circle represents all possible states of normal and shear stress on any plane through a stresses point in a material. Further we have seen that the co-ordinates of the point ‘Q' are seen to be the same as those derived from equilibrium of the element. i.e. the normal and shear stress components on any plane passing through the point can be found using Mohr's circle. Worthy of note: 1. The sides AB and BC of the element ABCD, which are 900 apart, are represented on the circle by and they are 1800 apart. 2. It has been shown that Mohr's circle represents all possible states at a point. Thus, it can be seen at a point. Thus, it, can be seen that two planes LP and PM, 1800 apart on the diagram and therefore 900 apart in the material, on which shear stress is zero. These planes are termed as principal planes and normal stresses acting on them are known as principal stresses. Thus , 1 = OL 2 = OM 3. The maximum shear stress in an element is given by the top and bottom points of the circle i.e by points J1 and J2 ,Thus the maximum shear stress would be equal to the radius of i.e. max= 1/2(12 ),the corresponding normal stress is obviously the distance OP = 1/2 (x+ y ) ,
- 42. Further it can also be seen that the planes on which the shear stress is maximum are situated 900 from the principal planes ( on circle ), and 450 in the material. 4.The minimum normal stress is just as important as the maximum. The algebraic minimum stress could have a magnitude greater than that of the maximum principal stress if the state of stress were such that the centre of the circle is to the left of orgin. i.e. if 1 = 20 MN/m2 (say) 2 = 80 MN/m2 (say) Then max m = ( 1 2 / 2 ) = 50 MN/m2 If should be noted that the principal stresses are considered a maximum or minimum mathematically e.g. a compressive or negative stress is less than a positive stress, irrespective or numerical value. 5. Since the stresses on perpendular faces of any element are given by the co-ordinates of two diametrically opposite points on the circle, thus, the sum of the two normal stresses for any and all orientations of the element is constant, i.e. Thus sum is an invariant for any particular state of stress. Sum of the two normal stress components acting on mutually perpendicular planes at a point in a state of plane stress is not affected by the orientation of these planes. This can be also understand from the circle Since AB and BC are diametrically opposite thus, what ever may be their orientation, they will always lie on the diametre or we can say that their sum won't change, it can also be seen from analytical relations
- 43. We know on plane BC; = 0 n1 = x on plane AB; = 2700 n2 = y Thus n1 + n2= x+ y 6. If 1 = 2, the Mohr's stress circle degenerates into a point and no shearing stresses are developed on xy plane. 7. If x+ y= 0, then the center of Mohr's circle coincides with the origin of co-ordinates.
- 44. ANALYSIS OF STRAINS CONCEPT OF STRAIN Concept of strain : if a bar is subjected to a direct load, and hence a stress the bar will change in length. If the bar has an original length L and changes by an amount L, the strain produce is defined as follows: Strain is thus, a measure of the deformation of the material and is a nondimensional Quantity i.e. it has no units. It is simply a ratio of two quantities with the same unit. Since in practice, the extensions of materials under load are very very small, it is often convenient to measure the strain in the form of strain x 10-6 i.e. micro strain, when the symbol used becomes . Sign convention for strain: Tensile strains are positive whereas compressive strains are negative. The strain defined earlier was known as linear strain or normal strain or the longitudinal strain now let us define the shear strain. Definition: An element which is subjected to a shear stress experiences a deformation as shown in the figure below. The tangent of the angle through which two adjacent sides rotate relative to their initial position is termed shear strain. In many cases the angle is very small and the angle it self is used, ( in radians ), instead of tangent, so that = AOB - A'OB' = Shear strain: As we know that the shear stresses acts along the surface. The action of the stresses is to produce or being about the deformation in the body consider the distortion produced b shear sheer stress on an element or rectangular block
- 45. This shear strain or slide is and can be defined as the change in right angle. or The angle of deformation is then termed as the shear strain. Shear strain is measured in radians & hence is non – dimensional i.e. it has no unit.So we have two types of strain i.e. normal stress & shear stresses. Hook's Law : A material is said to be elastic if it returns to its original, unloaded dimensions when load is removed. Hook's law therefore states that Stress () strain( ) Modulus of elasticity : Within the elastic limits of materials i.e. within the limits in which Hook's law applies, it has been shown that Stress / strain = constant This constant is given by the symbol E and is termed as the modulus of elasticity or Young's modulus of elasticity Thus The value of Young's modulus E is generally assumed to be the same in tension or compression and for most engineering material has high, numerical value of the order of 200 GPa
- 46. Poisson's ratio: If a bar is subjected to a longitudinal stress there will be a strain in this direction equal toE . There will also be a strain in all directions at right angles to . The final shape being shown by the dotted lines. It has been observed that for an elastic materials, the lateral strain is proportional to the longitudinal strain. The ratio of the lateral strain to longitudinal strain is known as the poison's ratio . Poison's ratio () = lateral strain / longitudinal strain For most engineering materials the value of his between 0.25 and 0.33. Three – dimensional state of strain : Consider an element subjected to three mutually perpendicular tensile stresses x , yand z as shown in the figure below. If y and z were not present the strain in the x direction from the basic definition of Young's modulus of Elasticity E would be equal to x= x/ E The effects of y and z in x direction are given by the definition of Poisson's ratio ‘ ' to be equal as y/ E and z/ E The negative sign indicating that if yand z are positive i.e. tensile, these they tend to reduce the strain in x direction thus the total linear strain is x direction is given by
- 47. Principal strains in terms of stress: In the absence of shear stresses on the faces of the elements let us say that x , y , z are in fact the principal stress. The resulting strain in the three directions would be the principal strains. i.e. We will have the following relation. For Two dimensional strain: system, the stress in the third direction becomes zero i.e z = 0 or 3 = 0 Although we will have a strain in this direction owing to stresses 1& 2 . Hence the set of equation as described earlier reduces to Hence a strain can exist without a stress in that direction
- 48. Hydrostatic stress : The term Hydrostatic stress is used to describe a state of tensile or compressive stress equal in all directions within or external to a body. Hydrostatic stress causes a change in volume of a material, which if expressed per unit of original volume gives a volumetric strain denoted byv. So let us determine the expression for the volumetric strain. Volumetric Strain: Consider a rectangle solid of sides x, y and z under the action of principal stresses 1 , 2 , 3 respectively. Then 1 , 2 , and 3 are the corresponding linear strains, than the dimensions of the rectangle becomes ( x + 1 . x ); ( y + 2 . y ); ( z + 3 . z ) hence the ALITER : Let a cuboid of material having initial sides of Length x, y and z. If under some load system, the sides changes in length by dx, dy, and dz then the new volume ( x + dx ) ( y + dy ) ( z +dz ) New volume = xyz + yzdx + xzdy + xydz Original volume = xyz Change in volume = yzdx +xzdy + xydz Volumetric strain = ( yzdx +xzdy + xydz ) / xyz = x+ y+ z Neglecting the products of epsilon's since the strains are sufficiently small.
- 49. Volumetric strains in terms of principal stresses: As we know that Strains on an oblique plane (a) Linear strain Consider a rectangular block of material OLMN as shown in the xy plane. The strains along ox and oy are x and y , and xy is the shearing strain. Then it is required to find an expression for , i.e the linear strain in a direction inclined at to OX, in terms of x ,y , xy and . Let the diagonal OM be of length 'a' then ON = a cos and OL = a sin , and the increase in length of those under strains arexacos and ya sin ( i.e. strain x original length ) respectively. If M moves to M', then the movement of M parallel to x axis is xacos + xy sin and the movement parallel to the y axis is yasin
- 50. Thus the movement of M parallel to OM , which since the strains are small is practically coincident with MM'. and this would be the summation of portions (1) and (2) respectively and is equal to This expression is identical in form with the equation defining the direct stress on any inclined plane with x and y replacing x and y and ½ xyreplacing xy i.e. the shear stress is replaced by half the shear strain Shear strain: To determine the shear stain in the direction OM consider the displacement of point P at the foot of the perpendicular from N to OM and the following expression can be derived as In the above expression ½ is there so as to keep the consistency with the stress relations. Futher -ve sign in the expression occurs so as to keep the consistency of sign convention, because OM' moves clockwise with respect to OM it is considered to be negative strain. The other relevant expressions are the following :
- 51. Let us now define the plane strain condition Plane Strain : In xy plane three strain components may exist as can be seen from the following figures: Therefore, a strain at any point in body can be characterized by two axial strains i.e x in x direction, y in y - direction and xy the shear strain. In the case of normal strains subscripts have been used to indicate the direction of the strain, and x , y are defined as the relative changes in length in the co-ordinate directions. With shear strains, the single subscript notation is not practical, because such strains involves displacements and length which are not in same direction.The symbol and subscript xy used for the shear strain referred to the x and y planes. The order of the subscript is unimportant. xy and yxrefer to the same physical quantity. However, the sign convention is important.The shear strain xy is considered to be positive if it represents a decrease the angle between the sides of an element of material lying parallel the positive x and y axes. Alternatively we can think of positive shear strains produced by the positive shear stresses and viceversa. Plane strain : An element of material subjected only to the strains as shown in Fig. 1, 2, and 3 respectively is termed as the plane strain state. Thus, the plane strain condition is defined only by the componentsx ,y , xy :z = 0;xz= 0; yz= 0
- 52. It should be noted that the plane stress is not the stress system associated with plane strain. The plane strain condition is associated with three dimensional stress system and plane stress is associated with three dimensional strain system.
- 53. PRINCIPAL STRAIN For the strains on an oblique plane we have an oblique we have two equations which are identical in form with the equation defining the direct stress on any inclined plane . Since the equations for stress and strains on oblique planes are identical in form, so it is evident that Mohr's stress circle construction can be used equally well to represent strain conditions using the horizontal axis for linear strains and the vertical axis for half the shear strain. It should be noted, however that the angles given by Mohr's stress circle refer to the directions of the planes on which the stress act and not the direction of the stresses themselves. The direction of the stresses and therefore associated strains are therefore normal (i.e. at 900 ) to the directions of the planes. Since angles are doubled in Mohr's stress circle construction it follows therefore that for a true similarity of working a relative rotation of axes of 2 x 900 = 1800 must be introduced. This is achieved by plotting positive sheer strains vertically downwards on the strain circle construction. The sign convention adopted for the strains is as follows: Linear Strains : extension - positive compression - negative { Shear of strains are taken positive, when they increase the original right angle of an unstrained element. } Shear strains : for Mohr's strains circle sheer strain xy - is +ve referred to x - direction the convention for the shear strains are bit difficult. The first subscript in the symbol xy usually denotes the shear strains associated with direction. e.g. in xy– represents the shear strain in x - direction and foryx– represents the shear strain in y - direction. If under strain the line associated with first subscript moves counter clockwise with respect to the other line, the shearing strain is said to be positive, and if it moves clockwise it is said to be negative. N.B: The positive shear strain is always to be drown on the top ofx .If the shear stain xy is given ] Moh's strain circle For the plane strain conditions can we derivate the following relations
- 54. A typical point P on the circle given the normal strain and half the sheer strain 1/2xy associated with a particular plane. We note again that an angle subtended at the centre of Mohr's circle by an arc connecting two points on the circle is twice the physical angle in the material. Mohr strain circle : Since the transformation equations for plane strain are similar to those for plane stress, we can employ a similar form of pictorial representation. This is known as Mohr's strain circle. The main difference between Mohr's stress circle and stress circle is that a factor of half is attached to the shear strains.
- 55. Points X' and Y' represents the strains associated with x and y directions with and xy /2 as co- ordiantes Co-ordinates of X' and Y' points are located as follows : In x – direction, the strains produced, the strains produced by x,and xy are x and xy /2 where as in the Y - direction, the strains are produced by y and + xy are produced by y and + xy These co-ordinated are consistent with our sign notation ( i.e. + ve shear stresses produces produce +ve shear strain & vice versa ) on the face AB is xy+ve i.e strains are ( y, +xy /2 ) where as on the face BC,xy is negative hence the strains are (x xy /2 )
- 56. A typical point P on the circle gives the normal strains and half the shear strain, associated with a particular plane we must measure the angle from x – axis (taken as reference) as the required formulas for ,1/2 have been derived with reference to x-axis with angle measuring in the c.c.W direction CONSTRUCTION : In this we would like to locate the points x' & y' instead of AB and BC as we have done in the case of Mohr's stress circle. steps 1. Take normal or linear strains on x-axis, whereas half of shear strains are plotted on y-axis. 2. Locate the points x' and y' 3. Join x' and y' and draw the Mohr's strain circle 4. Measure the required parameter from this construction.
- 57. Note: positive shear strains are associated with planes carrying positive shear stresses and negative strains with planes carrying negative shear stresses. ILLUSTRATIVE EXAMPLES : 1. At a certain point, a material is subjected to the following state of strains: x = 400 x 10-6 units y = 200 x 10-6 units xy = 350 x 10-6 radians Determine the magnitudes of the principal strains, the direction of the principal strains axes and the strain on an axis inclined at 300 clockwise to the x – axis. Solution: Draw the Mohr's strain circle by locating the points x' and y'
- 58. By Measurement the following values may be computed 1 = 500 X 10-6 units 2 = 100 x 10-6 units 1 = 600 /2 = 300 2 = 90 + 30 = 120 30 = 200 x 10-6 units The angles being measured c.c.w. from the direction of x. PROB 2. A material is subjected to two mutually perpendicular strains x = 350 x10-6 units and y = 50 x 10-6 units together with an unknown sheer strain xyif the principal strain in the material is 420 x 10-6 units Determine the following. (a) Magnitude of the shear strain (b) The other principal strain (c) The direction of principal strains axes (d) The magnitude of the principal stresses If E = 200 GN / m2 ;= 0.3
- 59. Solution : The Mohr's strain circle can be drawn as per the procedure described earlier. from the graphical construction, the following results may bre obtained : (i) Shear strain xy = 324 x 10-6 radians (ii) other principal strain = -20 x 10-6 (iii) direction of principal strain = 470 / 2 = 230 30' (iv) direction of other principal strain = 900 +230 30' = 1130 30' In order to determine the magnitude of principle stresses, the computed values of 1and 2 from the graphical construction may be substituted in the following expressions Use of strain Gauges : Although we can not measure stresses within a structural member, we can measure strains, and from them the stresses can be computed, Even so, we can only measure strains on the surface. For example, we can mark points and lines on the surface and measure changes in their spacing angles. In doing this we are of course only measuring average strains over the region concerned. Also in view of the very small changes in dimensions, it is difficult to archive accuracy in the measurements In practice, electrical strain gage provide a more accurate and convenient method of measuring strains. A typical strain gage is shown below.
- 60. The gage shown above can measure normal strain in the local plane of the surface in the direction of line PQ, which is parallel to the folds of paper. This strain is an average value of for the region covered by the gage, rather than a value at any particular point. The strain gage is not sensitive to normal strain in the direction perpendicular to PQ, nor does it respond to shear strain. therefore, in order to determine the state of strain at a particular small region of the surface, we usually need more than one strain gage. To define a general two dimensional state of strain, we need to have three pieces of information, such asx ,y and xy referred to any convenient orthogonal co-ordinates x and y in the plane of the surface. We therefore need to obtain measurements from three strain gages. These three gages must be arranged at different orientations on the surface to from a strain rossett. Typical examples have been shown, where the gages are arranged at either 450 or 600 to each other as shown below : A group of three gages arranged in a particular fashion is called a strain rosette. Because the rosette is mounted on the surface of the body, where the material is in plane stress, therefore, the transformation equations for plane strain to calculate the strains in various directions. Knowing the orientation of the three gages forming a rosette, together with the in – plane normal strains they record, the state of strain at the region of the surface concerned can be found. Let us consider the general case shown in the figure below, where three strain gages numbered 1,
- 61. 2, 3, where three strain gages numbered 1, 2, 3 are arranged at an angles of 1 , 2 , 3 measured c.c.w from reference direction, which we take as x – axis. Now, although the conditions at a surface, on which there are no shear or normal stress components. Are these of plane stress rather than the plane strain, we can still use strain transformation equations to express the three measured normal strains in terms of strain components x , y ,z and xy referred to x and y co-ordiantes as This is a set of three simultaneous linear algebraic equations for the three unknows x,y , xy to solve these equation is a laborious one as far as manually is concerned, but with computer it can be readily done.Using these later on, the state of strain can be determined at any point. Let us consider a 450 degree stain rosette consisting of three electrical – resistance strain gages arranged as shown in the figure below :
- 62. The gages A, B,C measure the normal strainsa , b , c in the direction of lines OA, OB and OC. Thus Thus, substituting the relation (3) in the equation (2) we get xy = 2b( a + c ) and other equation becomes x = a ; y= c Since the gages A and C are aligned with the x and y axes, they give the strains x and y directly Thus, x , y and xy can easily be determined from the strain gage readings. Knowing these strains, we can calculate the strains in any other directions by means of Mohr's circle or from the transformation equations. The 600 Rossett: For the 600 strain rosette, using the same procedure we can obtain following relation.
- 63. STRESS - STRAIN RELATIONS Stress – Strain Relations: The Hook's law, states that within the elastic limits the stress is proportional to the strain since for most materials it is impossible to describe the entire stress – strain curve with simple mathematical expression, in any given problem the behavior of the materials is represented by an idealized stress – strain curve, which emphasizes those aspects of the behaviors which are most important is that particular problem. (i) Linear elastic material: A linear elastic material is one in which the strain is proportional to stress as shown below: There are also other types of idealized models of material behavior. (ii) Rigid Materials: It is the one which donot experience any strain regardless of the applied stress.
- 64. (iii) Perfectly plastic(non-strain hardening): A perfectly plastic i.e non-strain hardening material is shown below: (iv) Rigid Plastic material(strain hardening): A rigid plastic material i.e strain hardening is depicted in the figure below: (v) Elastic Perfectly Plastic material: The elastic perfectly plastic material is having the characteristics as shown below:
- 65. (vi) Elastic – Plastic material: The elastic plastic material exhibits a stress Vs strain diagram as depicted in the figure below: Elastic Stress – strain Relations : Previously stress – strain relations were considered for the special case of a uniaxial loading i.e. only one component of stress i.e. the axial or normal component of stress was coming into picture. In this section we shall generalize the elastic behavior, so as to arrive at the relations which connect all the six components of stress with the six components of elastic stress. Futher, we would restrict overselves to linearly elastic material. Before writing down the relations let us introduce a term ISOTROPY ISOTROPIC: If the response of the material is independent of the orientation of the load axis of the sample, then we say that the material is isotropic or in other words we can say that isotropy of a material in a characteristics, which gives us the information that the properties are the same in the three orthogonal directions x y z, on the other hand if the response is dependent on orientation it is known as anisotropic. Examples of anisotropic materials, whose properties are different in different directions are (i) Wood (ii) Fibre reinforced plastic (iii) Reinforced concrete HOMOGENIUS: A material is homogenous if it has the same composition through our body. Hence the elastic properties are the same at every point in the body. However, the properties need not to be the same in all the direction for the material to be homogenous. Isotropic materials have the same elastic properties in all the directions. Therefore, the material must be both homogenous and isotropic in order to have the lateral strains to be same at every point in a particular component.
- 66. Generalized Hook's Law: We know that for stresses not greater than the proportional limit. These equation expresses the relationship between stress and strain (Hook's law) for uniaxial state of stress only when the stress is not greater than the proportional limit. In order to analyze the deformational effects produced by all the stresses, we shall consider the effects of one axial stress at a time. Since we presumably are dealing with strains of the order of one percent or less. These effects can be superimposed arbitrarily. The figure below shows the general triaxial state of stress. Let us consider a case when x alone is acting. It will cause an increase in dimension in X- direction whereas the dimensions in y and z direction will be decreased. Therefore the resulting strains in three directions are
- 67. Similarly let us consider that normal stress y alone is acting and the resulting strains are Now let us consider the stress z acting alone, thus the strains produced are
- 68. In the following analysis shear stresses were not considered. It can be shown that for an isotropic material's a shear stress will produce only its corresponding shear strain and will not influence the axial strain. Thus, we can write Hook's law for the individual shear strains and shear stresses in the following manner. The Equations (1) through (6) are known as Generalized Hook's law and are the constitutive equations for the linear elastic isotropic materials. When these equations isotropic materials. When these equations are used as written, the strains can be completely determined from known values of the stresses. To engineers the plane stress situation is of much relevance ( i.e. z = xz = yz = 0 ), Thus then the above set of equations reduces to Hook's law is probably the most well known and widely used constitutive equations for an engineering materials.” However, we can not say that all the engineering materials are linear elastic isotropic ones. Because now in the present times, the new materials are being developed every day. Many useful materials exhibit nonlinear response and are not elastic too.
- 69. Plane Stress: In many instances the stress situation is less complicated for example if we pull one long thin wire of uniform section and examine – small parallepiped where x – axis coincides with the axis of the wire So if we take the xy plane then x , y , xy will be the only stress components acting on the parrallepiped. This combination of stress components is called the plane stress situation A plane stress may be defined as a stress condition in which all components associated with a given direction ( i.e the z direction in this example ) are zero Plane strain: If we focus our attention on a body whose particles all lie in the same plane and which deforms only in this plane. This deforms only in this plane. This type of deformation is called as the plane strain, so for such a situation. z= zx = zy = 0 and the non – zero terms would be x, y & xy i.e. if strain components x, y and xy and angle are specified, the strain components x', y' and xy' with respect to some other axes can be determined.
- 70. ELASTIC CONSTANTS In considering the elastic behavior of an isotropic materials under, normal, shear and hydrostatic loading, we introduce a total of four elastic constants namely E, G, K, and . It turns out that not all of these are independent to the others. In fact, given any two of them, the other two can be foundout . Let us define these elastic constants (i) E = Young's Modulus of Rigidity = Stress / strain (ii) G = Shear Modulus or Modulus of rigidity = Shear stress / Shear strain (iii) = Possion's ratio = lateral strain / longitudinal strain (iv) K = Bulk Modulus of elasticity = Volumetric stress / Volumetric strain Where Volumetric strain = sum of linear stress in x, y and z direction. Volumetric stress = stress which cause the change in volume. Let us find the relations between them
- 71. RELATION AMONG ELASTIC CONSTANTS Relation between E, G and : Let us establish a relation among the elastic constants E,G and . Consider a cube of material of side ‘a' subjected to the action of the shear and complementary shear stresses as shown in the figure and producing the strained shape as shown in the figure below. Assuming that the strains are small and the angle A C B may be taken as 450 . Therefore strain on the diagonal OA = Change in length / original length Since angle between OA and OB is very small hence OA OB therefore BC, is the change in the length of the diagonal OA
- 72. Now this shear stress system is equivalent or can be replaced by a system of direct stresses at 450 as shown below. One set will be compressive, the other tensile, and both will be equal in value to the applied shear strain. Thus, for the direct state of stress system which applies along the diagonals:
- 73. We have introduced a total of four elastic constants, i.e E, G, K and . It turns out that not all of these are independent of the others. Infact given any two of then, the other two can be found. irrespective of the stresses i.e, the material is incompressible. When = 0.5 Value of k is infinite, rather than a zero value of E and volumetric strain is zero, or in other words, the material is incompressible. Relation between E, K and : Consider a cube subjected to three equal stresses as shown in the figure below The total strain in one direction or along one edge due to the application of hydrostatic stress or volumetric stress is given as
- 74. Relation between E, G and K : The relationship between E, G and K can be easily determained by eliminating from the already derived relations E = 2 G ( 1 + ) and E = 3 K ( 1 ) Thus, the following relationship may be obtained Relation between E, K and : From the already derived relations, E can be eliminated
- 75. Engineering Brief about the elastic constants : We have introduced a total of four elastic constants i.e E, G, K and . It may be seen that not all of these are independent of the others. Infact given any two of them, the other two can be determined. Futher, it may be noted that hence if = 0.5, the value of K becomes infinite, rather than a zero value of E and the volumetric strain is zero or in otherwords, the material becomes incompressible Futher, it may be noted that under condition of simple tension and simple shear, all real materials tend to experience displacements in the directions of the applied forces and Under hydrostatic loading they tend to increase in volume. In otherwords the value of the elastic constants E, G and K cannot be negative Therefore, the relations E = 2 G ( 1 + ) E = 3 K ( 1 ) Yields
- 76. In actual practice no real material has value of Poisson's ratio negative . Thus, the value of cannot be greater than 0.5, if however 0.5 than v =ve, which is physically unlikely because when the material is stretched its volume would always increase. Determination of Poisson's ratio: Poisson's ratio can be determined easily by simultaneous use of two strain gauges on a test specimen subjected to uniaxial tensile or compressive load. One gage is mounted parallel to the longitudnal axis of the specimen and other is mounted perpendicular to the longitudnal axis as shown below:
- 77. MECHANICAL PROPERTIES Mechanical Properties: In the course of operation or use, all the articles and structures are subjected to the action of external forces, which create stresses that inevitably cause deformation. To keep these stresses, and, consequently deformation within permissible limits it is necessary to select suitable materials for the Components of various designs and to apply the most effective heat treatment. i.e. a Comprehensive knowledge of the chief character tics of the semi-finished metal products & finished metal articles (such as strength, ductility, toughness etc) are essential for the purpose. For this reason the specification of metals, used in the manufacture of various products and structure, are based on the results of mechanical tests or we say that the mechanical tests conducted on the specially prepared specimens (test pieces) of standard form and size on special machines to obtained the strength, ductility and toughness characteristics of the metal. The conditions under which the mechanical test are conducted are of three types (1) Static: When the load is increased slowly and gradually and the metal is loaded by tension, compression, torsion or bending. (2) Dynamic: when the load increases rapidly as in impact (3) Repeated or Fatigue: (both static and impact type) . i.e. when the load repeatedly varies in the course of test either in value or both in value and direction Now let us consider the uniaxial tension test. [ For application where a force comes on and off the structure a number of times, the material cannot withstand the ultimate stress of a static tool. In such cases the ultimate strength depends on no. of times the force is applied as the material works at a particular stress level. Experiments one conducted to compute the number of cycles requires to break to specimen at a particular stress when fatigue or fluctuating load is acting. Such tests are known as fatque tests ] Uniaxial Tension Test: This test is of static type i.e. the load is increased comparatively slowly from zero to a certain value. Standard specimen's are used for the tension test. There are two types of standard specimen's which are generally used for this purpose, which have been shown below:
- 78. Specimen I: This specimen utilizes a circular X-section. Specimen II: This specimen utilizes a rectangular X-section. lg = gauge length i.e. length of the specimen on which we want to determine the mechanical properties.The uniaxial tension test is carried out on tensile testing machine and the following steps are performed to conduct this test. (i) The ends of the specimen's are secured in the grips of the testing machine. (ii) There is a unit for applying a load to the specimen with a hydraulic or mechanical drive. (iii) There must be a some recording device by which you should be able to measure the final output in the form of Load or stress. So the testing machines are often equipped with the pendulum type lever, pressure gauge and hydraulic capsule and the stress Vs strain diagram is plotted which has the following shape. A typical tensile test curve for the mild steel has been shown below
- 79. Nominal stress – Strain OR Conventional Stress – Strain diagrams: Stresses are usually computed on the basis of the original area of the specimen; such stresses are often referred to as conventional or nominal stresses. True stress – Strain Diagram: Since when a material is subjected to a uniaxial load, some contraction or expansion always takes place. Thus, dividing the applied force by the corresponding actual area of the specimen at the same instant gives the so called true stress. SALIENT POINTS OF THE GRAPH: (A) So it is evident form the graph that the strain is proportional to strain or elongation is proportional to the load giving a st.line relationship. This law of proportionality is valid upto a point A. or we can say that point A is some ultimate point when the linear nature of the graph ceases or there is a deviation from the linear nature. This point is known as the limit of proportionality or the proportionality limit. (B) For a short period beyond the point A, the material may still be elastic in the sense that the deformations are completely recovered when the load is removed. The limiting point B is termed as Elastic Limit . (C) and (D) - Beyond the elastic limit plastic deformation occurs and strains are not totally recoverable. There will be thus permanent deformation or permanent set when load is removed. These two points are termed as upper and lower yield points respectively. The stress at the yield point is called the yield strength. A study a stress – strain diagrams shows that the yield point is so near the proportional limit that for most purpose the two may be taken as one. However, it is much easier to locate the former.
- 80. For material which do not posses a well define yield points, In order to find the yield point or yield strength, an offset method is applied. In this method a line is drawn parallel to the straight line portion of initial stress diagram by off setting this by an amount equal to 0.2% of the strain as shown as below and this happens especially for the low carbon steel. (E) A further increase in the load will cause marked deformation in the whole volume of the metal. The maximum load which the specimen can with stand without failure is called the load at the ultimate strength. The highest point ‘E' of the diagram corresponds to the ultimate strength of a material. u = Stress which the specimen can with stand without failure & is known as Ultimate Strength or Tensile Strength. u is equal to load at E divided by the original cross-sectional area of the bar. (F) Beyond point E, the bar begins to forms neck. The load falling from the maximum until fracture occurs at F. [ Beyond point E, the cross-sectional area of the specimen begins to reduce rapidly over a relatively small length of bar and the bar is said to form a neck. This necking takes place whilst the load reduces, and fracture of the bar finally occurs at point F ] Note: Owing to large reduction in area produced by the necking process the actual stress at fracture is often greater than the above value. Since the designers are interested in maximum loads which can be carried by the complete cross section, hence the stress at fracture is seldom of any practical value.
- 81. Percentage Elongation: ' ': The ductility of a material in tension can be characterized by its elongation and by the reduction in area at the cross section where fracture occurs. It is the ratio of the extension in length of the specimen after fracture to its initial gauge length, expressed in percent. lI = gauge length of specimen after fracture(or the distance between the gage marks at fracture) lg= gauge length before fracture(i.e. initial gauge length) For 50 mm gage length, steel may here a % elongation of the order of 10% to 40%. Elastic Action: The elastic is an adjective meaning capable of recovering size and shape after deformation. Elastic range is the range of stress below the elastic limit. Many engineering materials behave as indicated in Fig(a) however, some behaves as shown in figures in (b) and (c) while in elastic range. When a material behaves as in (c), the vs is not single valued since the strain corresponding to any particular ‘ ' will depend upon loading history. Fig (d): It illustrates the idea of elastic and plastic strain. If a material is stressed to level (1) and then relased the strain will return to zero beyond this plastic deformation remains.
- 82. If a material is stressed to level (2) and then released, the material will recover the amount (2 2p ), where 2p is the plastic strain remaining after the load is removed. Similarly for level (3) the plastic strain will be3p. Ductile and Brittle Materials: Based on this behaviour, the materials may be classified as ductile or brittle materials Ductile Materials: It we just examine the earlier tension curve one can notice that the extension of the materials over the plastic range is considerably in excess of that associated with elastic loading. The Capacity of materials to allow these large deformations or large extensions without failure is termed as ductility. The materials with high ductility are termed as ductile materials. Brittle Materials: A brittle material is one which exhibits a relatively small extensions or deformations to fracture, so that the partially plastic region of the tensile test graph is much reduced. This type of graph is shown by the cast iron or steels with high carbon contents or concrete. Conditions Affecting Mechanical Properties: The Mechanical properties depend on the test conditions (1) It has been established that lowering the temperature or increasing the rate of deformation considerably increases the resistance to plastic deformation. Thus, at low temperature (or higher rates of deformation), metals and alloys, which are ductile at normal room temperature may fail with brittle fracture. (2) Notches i.e. sharp charges in cross sections have a great effect on the mechanical properties of the metals. A Notch will cause a non – uniform distribution of stresses. They will always contribute lowering the ductility of the materials. A notch reduces the ultimate strength of the high strength materials. Because of the non – uniform distribution of the stress or due to stress concentration.
- 83. (3) Grain Size : The grain size also affects the mechanical properties. Hardness: Hardness is the resistance of a metal to the penetration of another harder body which does not receive a permanent set. Hardness Tests consists in measuring the resistance to plastic deformation of layers of metals near the surface of the specimen i.e. there are Ball indentation Tests. Ball indentation Tests: iThis method consists in pressing a hardened steel ball under a constant load P into a specially prepared flat surface on the test specimen as indicated in the figures below : After removing the load an indentation remains on the surface of the test specimen. If area of the spherical surface in the indentation is denoted as F sq. mm. Brinell Hardness number is defined as : Bhn = P / F F is expressed in terms of D and d D = ball diameter d = diametric of indentation and Brinell Hardness number is given by Then is there is also Vicker's Hardness Number in which the ball is of conical shape.
- 84. IMPACT STRENGTH Static tension tests of the unnotched specimen's do not always reveal the susceptibility of metal to brittle fracture. This important factor is determined in impact tests. In impact tests we use the notched specimen's this specimen is placed on its supports on anvil so that blow of the striker is opposite to the notch the impact strength is defined as the energy A, required to rupture the specimen, Impact Strength = A / f Where f = It is the cross – section area of the specimen in cm2 at fracture & obviously at notch. The impact strength is a complex characteristic which takes into account both toughness and strength of a material. The main purpose of notched – bar tests is to study the simultaneous effect of stress concentration and high velocity load application Impact test are of the severest type and facilitate brittle friction. Impact strength values can not be as yet be used for design calculations but these tests as rule provided for in specifications for carbon & alloy steels.Futher, it may be noted that in impact tests fracture may be either brittle or ductile. In the case of brittle fracture, fracture occurs by separation and is not accompanied by noticeable plastic deformation as occurs in the case of ductile fracture. Compression Test: Machines used for compression testing are basically similar to those used for tensile testing often the same machine can be used to perform both tests. Shape of the specimen: The shape of the machine to be used for the different materials are as follows: (i) For metals and certain plastics: The specimen may be in the from of a cylinder (ii) For building materials: Such as concrete or stone the shape of the specimen may be in the from of a cube. Shape of stress stain diagram (a) Ductile materials: For ductile material such as mild steel, the load Vs compression diagram would be as follows
- 85. (1) The ductile materials such as steel, Aluminum, and copper have stress – strain diagrams similar to ones which we have for tensile test, there would be an elastic range which is then followed by a plastic region. (2) The ductile materials (steel, Aluminum, copper) proportional limits in compression test are very much close to those in tension. (3) In tension test, a specimen is being stretched, necking may occur, and ultimately fracture fakes place. On the other hand when a small specimen of the ductile material is compressed, it begins to bulge on sides and becomes barrel shaped as shown in the figure above. With increasing load, the specimen is flattened out, thus offering increased resistance to further shortening ( which means that the stress – strains curve goes upward ) this effect is indicated in the diagram. Brittle materials ( in compression test ) Brittle materials in compression typically have an initial linear region followed by a region in which the shortening increases at a higher rate than does the load. Thus, the compression stress – strain diagram has a shape that is similar to the shape of the tensile diagram. However, brittle materials usually reach much higher ultimate stresses in compression than in tension. For cast iron, the shape may be like this
- 86. Brittle materials in compression behave elastically up to certain load, and then fail suddenly by splitting or by craking in the way as shown in figure. The brittle fracture is performed by separation and is not accompanied by noticeable plastic deformation. Hardness Testing: The tem ‘hardness' is one having a variety of meanings; a hard material is thought of as one whose surface resists indentation or scratching, and which has the ability to indent or cut other materials. Hardness test: The hardness test is a comparative test and has been evolved mainly from the need to have some convenient method of measuring the resistance of materials to scratching, wear or in dentation this is also used to give a guide to overall strength of a materials, after as an inspection procedure, and has the advantage of being a non – destructive test, in that only small indentations are lift permanently on the surface of the specimen. Four hardness tests are customarily used in industry namely (i) Brinell (ii) Vickers (iii) Rockwell (vi) Shore Scleroscopy The most widely used are the first two. In the Brinell test the indenter is a hardened steel ball which is pressed into the surface using a known standard load. The diameter of resulting indentation is than measured using a microscope & scale. Units:
- 87. The units of Brinell Hardness number in S.I Unit would have been N/mm2 or Mpa To avoid the confusion which would have been caused of her wise Hardness numbers are quotes as kgf / mm2 Brinell Hardness test: In the Brinell hardness test, a hardened steel ball is pressed into the flat surface of a test piece using a specified force. The ball is then removed and the diameter of the resulting indentation is measured using a microscope. The Brinell Hardness no. ( BHN ) is defined as BHN = P / A Where P = Force applied to the ball. A = curved area of the indentation It may be shown that D = diameter of the ball, d = the diameter of the indentation. In the Brinell Test, the ball diameter and applied load are constant and are selected to suit the composition of the metal, its hardness, and selected to suit the composition of the metal, its hardness, the thickness etc. Further, the hardness of the ball should be at least 1.7 times than the test specimen to prevent permanent set in the ball. Disadvantage of Brinell Hardness Test: The main disadvantage of the Brinell Hardness test is that the Brinell hardness number is not independent of the applied load. This can be realized from. Considering the geometry of indentations for increasing loads. As the ball is pressed into the surface under increasing load the geometry of the indentation charges. Here what we mean is that the geometry of the impression should not change w.r.t. load, however the size it impression may change.
- 88. Vickers Hardness test: The Vicker's Hardness test follows a procedure exactly a identical with that of Brinell test, but uses a different indenter. The steel ball is replaced by a diamond, having the from of a square – based pyramid with an angle of 1360 between opposite faces. This is pressed into the flat surface of the test piece using a specified force, and the diagonals of the resulting indentation measured is using a microscope. The Hardness, expressed as a Vicker's pyramid number is defined as the ratio F/A, where F is the force applied to the diamond and A is the surface area of the indentation. It may be shown that In the Vicker Test the indenters of pyramidal or conical shape are used & this overcomes the disadvantage which is faced in Brinell test i.e. as the load increases, the geometry of the indentation's does not change
- 89. The Variation of Hardness number with load is given below. Advantage: Apart from the convenience the vicker's test has certain advantages over the Brinell test. (i) Harder material can be tested and indentation can be smaller & therefore less obtrusive or damaging. Upto a 300 kgf /mm2 both tests give the same hardness number but above too the Brinell test is unreliable. Rockwell Hardness Test : The Rockwell Hardness test also uses an indenter when is pressed into the flat surface of the test piece, but differs from the Brinell and Vicker's test in that the measurement of hardness is based on the depth of penetration, not on the surface area of indentation. The indenter may be a conical diamond of 1200 included angle, with a rounded apex. It is brought into contact with the test piece, and a force F is applied.
- 90. Advantages : Rockwell tests are widely applied in industry due to rapidity and simplicity with which they may be performed, high accuracy, and due to the small size of the impressions produced on the surface. Impact testing: In an ‘impact test' a notched bar of material, arranged either as a cantilever or as a simply supported beam, is broken by a single blow in such a way that the total energy required to fracture it may be determined. The energy required to fracture a material is of importance in cases of “shock loading' when a component or structure may be required to absorb the K.E of a moving object. Often a structure must be capable of receiving an accidental ‘shock load' without failing completely, and whether it can do this will be determined not by its strength but by its ability to absorb energy. A combination of strength and ductility will be required, since large amounts of energy can only be absorbed by large amounts of plastic deformation. The ability of a material to absorb a large amount of energy before breaking is often referred as toughness, and the energy absorbed in an impact test is an obvious indication of this property. Impact tests are carried out on notched specimens, and the notches must not be regarded simply as a local reduction in the cross – sectional area of the specimen, Notches – and , in fact, surface irregularities of many kind – give rise to high local stresses, and are in practice, a potential source of cracks. The specimen may be of circular or square cross – section arranged either as a cantilever or a simply supported beam.
- 91. Toughness: It is defined as the ability of the material to withstand crack i.e to prevent the transfer or propagation of cracks across its section hence causing failures. Cracks are propagated due to stress concentraction. Creep: Creep is the gradual increase of plastic strain in a material with time at constant load. Particularly at elevated temperatures some materials are susceptible to this phenomena and even under the constant load, mentioned strains can increase continually until fractures. This form of facture is particularly relevant to the turbines blades, nuclear rectors, furnaces rocket motors etc. The general from of strain versus time graph or creep curve is shown below. The general form of Vs t graph or creep curve is shown below for two typical operation conditions, In each case the curve can be considered to exhibit four principal features (a) An initial strain, due to the initial application of load. In most cases this would be an elastic strain. (b) A primary creep region, during which he creep rate ( slope of the graph ) dimensions. (c) A secondary creep region, when the creep rate is sensibly constant. (d) A tertiary creep region, during which the creep rate accelerate to final fracture. It is obvious that a material which is susceptible to creep effects should only be subjected to stresses which keep it in secondary (st.line) region throughout its service life. This enables the amount of creep extension to be estimated and allowed for in design. Practice Problems: PROB 1: A standard mild steel tensile test specimen has a diameter of 16 mm and a gauge length of 80 mm such a specimen was tested to destruction, and the following results obtained. Load at yield point = 87 kN
- 92. Extension at yield point = 173 x 166 m Ultimate load = 124 kN Total extension at fracture = 24 mm Diameter of specimen at fracture = 9.8 mm Cross - sectional area at fracture = 75.4 mm2 Cross - sectional Area ‘A' = 200 mm2 Compute the followings: (i) Modulus of elasticity of steel (ii) The ultimate tensile stream (iii) The yield stress (iv) The percentage elongation (v) The Percentage reduction in Area. PROB 2: A light alloy specimen has a diameter of 16mm and a gauge Length of 80 mm. When tested in tension, the load extension graph proved linear up to a load of 6kN, at which point the extension was 0.034 mm. Determine the limits of proportionality stress and the modulus of elasticity of material. Note: For a 16mm diameter specimen, the Cross – sectional area A = 200 mm2 This is according to tables Determine the limit of proportion try stream & the modulus of elasticity for the material. Ans: 30 MN /m2 , 70.5 GN /m2 solution:
- 93. Members Subjected to Uniaxial Stress Members in Uni – axial state of stress Introduction: [For members subjected to uniaxial state of stress] For a prismatic bar loaded in tension by an axial force P, the elongation of the bar can be determined as Suppose the bar is loaded at one or more intermediate positions, then equation (1) can be readily adapted to handle this situation, i.e. we can determine the axial force in each part of the bar i.e. parts AB, BC, CD, and calculate the elongation or shortening of each part separately, finally, these changes in lengths can be added algebraically to obtain the total charge in length of the entire bar. When either the axial force or the cross – sectional area varies continuosly along the axis of the bar, then equation (1) is no longer suitable. Instead, the elongation can be found by considering a deferential element of a bar and then the equation (1) becomes i.e. the axial force Pxand area of the cross – section Ax must be expressed as functions of x. If the expressions for Pxand Ax are not too complicated, the integral can be evaluated analytically, otherwise Numerical methods or techniques can be used to evaluate these integrals.
- 94. stresses in Non – Uniform bars Consider a bar of varying cross section subjected to a tensile force P as shown below. Let a = cross sectional area of the bar at a chosen section XX then Stress = p / a If E = Young's modulus of bar then the strain at the section XX can be calculated = / E Then the extension of the short element x. = .original length = / E. x Now let us for example take a case when the bar tapers uniformly from d at x = 0 to D at x = l
- 95. In order to compute the value of diameter of a bar at a chosen location let us determine the value of dimension k, from similar triangles therefore, the diameter 'y' at the X-section is or = d + 2k Hence the cross –section area at section X- X will be
- 96. hence the total extension of the bar will be given by expression An interesting problem is to determine the shape of a bar which would have a uniform stress in it under the action of its own weight and a load P. let us consider such a bar as shown in the figure below: The weight of the bar being supported under section XX is
- 97. The same results are obtained if the bar is turned upside down and loaded as a column as shown in the figure below:
- 98. IIIustrative Problem 1: Calculate the overall change in length of the tapered rod as shown in figure below. It carries a tensile load of 10kN at the free end and at the step change in section a compressive load of 2 MN/m evenly distributed around a circle of 30 mm diameter take the value of E = 208 GN / m2 . This problem may be solved using the procedure as discussed earlier in this section IIIustrative Problem 2: A round bar, of length L, tapers uniformly from radius r1 at one end to radius r2at the other. Show that the extension produced by a tensile axial load P is
- 99. If r2 = 2r1 , compare this extension with that of a uniform cylindrical bar having a radius equal to the mean radius of the tapered bar. Solution: consider the above figure let r1 be the radius at the smaller end. Then at a X crosssection XX located at a distance x from the smaller end, the value of radius is equal to
- 100. Comparing of extensions For the case when r2 = 2.r1, the value of computed extension as above becomes equal to The mean radius of taper bar = 1 / 2( r1 + r2 ) = 1 / 2( r1 +2 r2 ) = 3 / 2 .r1 Therefore, the extension of uniform bar = Orginal length . strain Thermal stresses, Bars subjected to tension and Compression Compound bar: In certain application it is necessary to use a combination of elements or bars made from different materials, each material performing a different function. In over head electric cables or Transmission Lines for example it is often convenient to carry the current in a set of copper wires surrounding steel wires. The later being designed to support the weight of the cable over large spans. Such a combination of materials is generally termed compound bars. Consider therefore, a compound bar consisting of n members, each having a different length and cross sectional area and each being of a different material. Let all member have a common extension ‘x' i.e. the load is positioned to produce the same extension in each member.
- 101. Where Fn is the force in the nth member and An and Ln are its cross - sectional area and length. Let W be the total load, the total load carried will be the sum of all loads for all the members. Therefore, each member carries a portion of the total load W proportional of EA / L value.
- 102. The above expression may be writen as if the length of each individual member in same then, we may write Thus, the stress in member '1' may be determined as 1 = F1 / A1 Determination of common extension of compound bars: In order to determine the common extension of a compound bar it is convenient to consider it as a single bar of an imaginary material with an equivalent or combined modulus Ec. Assumption: Here it is necessary to assume that both the extension and original lengths of the individual members of the compound bar are the same, the strains in all members will than be equal. Total load on compound bar = F1 + F2+ F3 +………+ Fn where F1 , F 2 ,….,etc are the loads in members 1,2 etc But force = stress . area,therefore (A 1 + A 2 + ……+ A n ) = 1 A1 + 2 A2 + ........+n An Where is the stress in the equivalent single bar Dividing throughout by the common strain.
- 103. Compound bars subjected to Temp. Change : Ordinary materials expand when heated and contract when cooled, hence , an increase in temperature produce a positive thermal strain. Thermal strains usually are reversible in a sense that the member returns to its original shape when the temperature return to its original value. However, there here are some materials which do not behave in this manner. These metals differs from ordinary materials in a sence that the strains are related non linearly to temperature and some times are irreversible .when a material is subjected to a change in temp. is a length will change by an amount. t = .L.t ort.L.t or t= E ..t = coefficient of linear expansoin for the material L = original Length t = temp. change Thus an increase in temperature produces an increase in length and a decrease in temperature results in a decrease in length except in very special cases of materials with zero or negative coefficients of expansion which need not to be considered here. If however, the free expansion of the material is prevented by some external force, then a stress is set up in the material. They stress is equal in magnitude to that which would be produced in the bar by initially allowing the bar to its free length and then applying sufficient force to return the bar to its original length. Change in Length = L t Therefore, strain = L t / L = t Therefore ,the stress generated in the material by the application of sufficient force to remove this strain = strain x E or Stress = E t Consider now a compound bar constructed from two different materials rigidly joined together, for simplicity. Let us consider that the materials in this case are steel and brass.
- 104. If we have both applied stresses and a temp. change, thermal strains may be added to those given by generalized hook's law equation –e.g. While the normal strains a body are affected by changes in temperatures, shear strains are not. Because if the temp. of any block or element changes, then its size changes not its shape therefore shear strains do not change. In general, the coefficients of expansion of the two materials forming the compound bar will be different so that as the temp. rises each material will attempt to expand by different amounts. Figure below shows the positions to which the individual materials will expand if they are completely free to expand (i.e not joined rigidly together as a compound bar). The extension of any Length L is given by L t In general, changes in lengths due to thermal strains may be calculated form equation t = Lt, provided that the members are able to expand or contract freely, a situation that exists in

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment